**ON THE EFFECT OF THE NUMBER OF ANNUAL GROWTH RINGS, **

**SPECIFIC GRAVITY AND TEMPERATURE ON **

**REDWOOD ELASTIC MODULUS**

**Nilson T.Mascia****1**_{, Steven M.Cramer}**2**

**ABSTRACT**

Due to the natural origin of wood, physical parameters such as specifi c gravity and the number of growth rings per inch affect its properties. In this study, to evaluate the effect that these physical para-meters have on the elastic properties of wood, particularly on elastic modulus, a uniaxial compression test was performed on specimens. These specimens consisted of solid cubes of the Redwood species of wood with a width of 10.16 cm. Three different temperature conditions—ambient temperature (18°C), cold temperature (-28°C) and hot temperature (65°C) were used to carry out the tests. Specifi c gravity ranged from 0.29 to 0.45, and the number of growth rings per inch varied from 2 to 24 rings per inch. The minimum moisture content in the specimens was 2%, and reached a maximum of 16% according to the temperature conditions. The results from the statistical analysis indicated that the effect that the number of growth rings per inch has on elastic modulus is more signifi cant than the effects of specifi c gravity or even of temperature. As a consequence, we suggest that the number of growth rings per inch can be used as a predictor for wood elastic modulus.

**Keywords: **Moisture content; number of annual growth rings per inch; specifi c gravity;
tempera-ture; wood elastic modulus.

**RESUMEN**

Debido al origen natural de la madera, parámetros físicos como la gravedad específi ca y el núme-ro de anillos de crecimiento afectan sus pnúme-ropiedades. En este estudio para evaluar el efecto que estos parámetros físicos tienen sobre las propiedades elásticas de la madera, particularmente en el módulo de elasticidad, ensayos de compresión uniaxial se realizaron en probetas normalizadas. Estos probetas consistieron en cubos sólidos de la especie de madera Redwood con arista de 10,16 cm. Tres diferentes condiciones de temperatura fueron utilizadas para llevar a cabo las pruebas: ambiente (18 °C), bajo cero (-28 °C) y temperado (65 °C). La gravedad específi ca osciló entre 0,29 a 0,45 y el número de anillos de crecimiento varió de 2 a 24 anillos por pulgada. El mínimo contenido de humedad en las muestras fue del 2% y alcanzó un máximo del 16% de acuerdo a las condiciones de temperatura. Los resultados del análisis estadístico indicaron que el efecto del número de anillos de crecimiento por pulgada es más importante que los efectos de la gravedad específi ca o incluso que el de la temperatura sobre el módulo de elasticidad. En consecuencia, se sugiere aquí que el número de anillos de crecimiento por pulgada pueda ser utilizado como predictor del módulo de elasticidad de la madera.

**Palabras clave: **Contenido de humedad, número de anillos de crecimiento anual por pulgada;

**INTRODUCTION**

Several pieces of research, including Bodig and Jayne (1982) and Dinwoodie (2000), have analy-zed the behavior of wood under a uniaxial stress fi eld to determine the elastic constants of the wood. In these analyses, the infl uences of physical parameters, such as moisture content and specifi c gravity, on the modulus of elasticity were considered.

Wood is a heterogeneous material whose properties depend greatly on the species, biological di-versity and growth conditions. Indeed, wood properties are affected by many parameters, including temperature, creep, knots, number of growth rings and grain angle.

The literature contains many analyses showing that moisture content signifi cantly affects the elastic constants of wood (Wood Handbook 1987). Similarly, there are several studies, for instance Gerhards (1982) and Lenth and Sargent (2004), showing that an increase in temperature results in a decrease in the elastic constants of wood. Since, changes in temperature imply changes in moisture content, both parameters are, in practice, often interrelated. Some studies, such as Dinwoodie (2000), also demons-trate that there is a high correlation between specifi c gravity and the elastic constants of wood.

The number of growth rings per inch also affects the modulus of elasticity; this is especially impor-tant when comparing the effects of specifi c gravity and different temperature conditions. This fact is not commonly presented in the literature and, as we will demonstrate in this paper, signifi cantly interferes with the values of the modulus of elasticity obtained.

The specifi c aim of this paper is to evaluate the infl uence of specifi c gravity and the number of an-nual growth rings on the Young´s modulus of wood. To do this, three different temperature conditions are applied, and the results of a compression test in Redwood specimens are analyzed, focused on the extensive statistical procedure. We also note that the moisture content of the specimens used in the tests varied according to the temperature, clearly altering the values of wood elastic modulus.

As a result of this research, we suggest that the number of growth rings per inch should be consi-dered good predictor of wood material properties.

**PARAMETERS THAT INFLUENCE WOOD ELASTIC CONSTANTS**

In this study we analyzed parameters that exert any infl uence on the wood elastic modulus. The literature regarding the infl uence of moisture content on the wood elastic constants,such as Gerhards (1982) and Hanhijiirvi (2000), states that if this parameter increases, the elastic moduli decrease, whe-reas the Poisson´s ratios incwhe-rease. These variations occur until the moisture content reaches the Fiber Saturation Point—around 27% to 30% for most species of wood.

In contrast, Dinwoodie (2000) and the U.S. Dept. of Agriculture’s Wood Handbook (1987) show that the elastic constants are increased by increasing specifi c gravity. In addition, procedures analyzing the effect of the specifi c gravity on the wood elastic constants show evidence of a high correlation bet-ween the specifi c gravity and the elastic constants for example, Ballarin and Palma (2003). This is due to the fact that specifi c gravity is a function of the ratio between cell wall thickness and cell diameter. This ratio is related to the stiffness of wood and consequently to the elastic modulus.

Focusing on the infl uence that temperature exerts wood properties, it has been described in techni-cal literature, for instance Bodig and Jayne (1982), that when temperature increases, the values of elas-tic parameters of wood decrease. Furthermore, changes in temperature infl uence changes in moisture

content. Dinwoodie (2000) highlights that when the moisture content is at 0% (dry condition) and the temperature varied between -20°C and +60°C, the reduction in stiffness is 6%. However, when mois-ture content reached 20%, the reduction in stiffness was approximately 40%. Lenth and Sargent (2004) obtained similar results studying the tensile stiffness of specimens of radiata pine.

In their study of the parameters that infl uence redwood crush, Cramer, Hermanson and McMurtry (1996) and Hermanson (1996) note that the number of growth rings per inch may, in some cases, pre-dict the crush behavior more effi ciently than the specifi c gravity. Therefore, by considering the number of rings, it is possible to take into account the actual differences in specimen microstructure of the Redwood species.

Using the fi nite element method, Ando and Ohta (1999) analyzed the effects that the location of the crack tip in an annual ring and the direction of crack propagation have on the fracture toughness of the TR crack propagation system of coniferous wood. This validated earlier fi ndings regarding the changes in elastic modulus and strength within an annual ring as, for instance, Bodig and Jayne (1982) showed results suggesting a variation in the tensile strength of wood within the location of the growth rings.

In light of these earlier fi ndings, it can be expected that since the elastic modulus and the strength have a strong statistical relationship, the number of growth rings per inch will also have a statistically signifi cant relation to elastic modulus. In the following, the relationship between the previously men-tioned parameters and the wood elastic modulus are evaluated.

**MATERIAL AND EXPERIMENTAL METHODS**

The experimental data used to analyze the modulus of elasticity and the parameters that infl uen-ce the elastic coeffi cients were obtained from S.M. Cramer and J.C. Hermanson at the University of Wisconsin-Madison, Hermanson (1996). Here, we present a summary of the experimental procedure.

38 specimens of Redwood species were used from a random sample. The specimens consisted of solid cubes with a width of 10.16 cm, fabricated from 15.24 cm by 15.24 cm lumber, 5.40 m to 6.60 m in length.

The fi ber orientations with respect to the applied vertical load varied from 0° to 5°. We used this range so that the fi ber directions would have no signifi cant effect on the values of the modulus of elas-ticity. We observe that many studies, such as Bodig and Jayne (1982), Dinwoodie (2000) or Mascia (2003), the effect of grain angle orientation on the elastic modulus constitutes the fundamental cause of wood anisotropy. It is responsible for the greatest changes in the values of the elastic constant values of wood.

Figure 1 illustrates this mechanical behavior of 101 values of elastic modulus (this sample includes specimens with fi ber directions varied from 0° to 90°) obtained by S.M. Cramer and J.C. Hermanson. It can be observed that the pattern of the nonlinear curve follows the constitutive equation for wood and also the previous cited studies provide more specifi c information.

**Figure 1. **Variation of Elastic modulus with the fi ber direction of wood.

The specifi c gravity varied between 0.29 and 0.41. The number of growth rings per inch were re-corded by photocopying the end of the specimen, and ranged from 2 to 24 growth rings per inch (2.54 cm).

Three different temperature conditions were used: an ambient temperature (18°C), a cold tempera-ture (-28°C) and a hot temperatempera-ture (65°C). In this experimental procedure, all specimens were equili-brated to approximately 13%, but according to the temperature conditions the moisture content varied between 2.3 and 15.7%.

The tests consisted of applying a vertical load to redwood cubes unconfi ned in an instrumental steel box as it is presented in Figure 2. The displacements were measured at the centroid of the specimens.

**Figure 2.** Schematic of triaxial test divice. (S.M. Cramer and J.C. Hermanson at University of
Wisconsin-Madison).

Just to exemplify, Table 1 contains the experimental data used in this work.

**RESULTS AND DISCUSSIONS**

In this analysis we developed fi ve comparisons to evaluate the infl uence that specifi c gravity, num-ber of growth rings per inch, and temperature associated to the moisture content have on Young´s modulus. To explore the number of growth rings per inch as a predictor for wood elastic modulus, we developed a relationship between this parameter and specifi c gravity, a known predictor of the elastic modulus of wood.

To carry out this study, we used a linear regression model, and closely analyzed the variance and the values that affect the adopted model.

Before presenting the statistical procedure, we note that the tested sample constitutes a normal
distribution, according to the Anderson-Darling test of normality (see Montgomery and Peck (1992)
or Ryan and Joiner (1994)), with mean η = 4156.3 MPa, and standard deviation σ = 974.6 MPa. These
results constituted a coeffi cient of variation (C*V*) of 0.23, a satisfactory value for experimental tests on
wood.

**Statistical analysis**

Following Montgomery and Peck (1992) and Ryan and Joiner (1994), the linear regression model
can generally be written as: *y = *β* _{0 }*+ β

*+ β*

_{1}x_{1}*+ ... + β*

_{2}x_{2 }*+ ε. It is supposed that the errors are normally and independently distributed with mean η= 0 and variance σ2*

_{k}x_{k }_{.}

The regression analysis can be summarized by verifying:

1. The test of the signifi cance of regression follows the hypothesis:.

*H _{0} : *β

*β*

_{1}=*β*

_{2}= ... =*β*

_{k}= 0 versus H_{1}:*≠β*

_{1}*≠*

_{2}*...*β

*≠*

_{k}*0*

The statistic is employed, implying that the hypothesis *H _{0} : *β

*β*

_{1}=*β*

_{2}= ... =

_{k}= 0is rejected at a desirable level of signifi cance, generally 5–15%. Thus, it is possible to accept or reject the linear model and we make inferences about β parameters that have practical signifi cance. In this case, the t-values for each coeffi cient in the model should be calculated.

Here, *n* is the number of pairs of data, *k* is the number of β parameters in the model (excluding

β* _{0}*), α is the level of signifi cance,

*t*

_{α}

*is the Student’s t-distribution and*

_{ /2, n-(k+1)}*n-(k+1)*are the degrees of freedom.

2. The analysis of variance is given by the following statistic:

, where *MS _{R}* is the regression mean square and

*MS*is the residual

_{E}mean square.

To test the hypothesis *H _{0} : *β

*β*

_{1}=*β*

_{2}= ... =*, we compute the statistical test*

_{k}= 0*F*and reject

_{0}*H _{0}* if

*F*>

_{0}*F*

_{α}

_{,(k,n-(k+1))}, with certain probability

*p*. The test procedure is summarized in Table 2. We can

observe that if the observed value of *F _{0}* is large, the parameter β

*is statistically different from zero, with probability*

_{k}*p*.

**Table 2.** Analysis of the Variance for Signifi cance of Regression

3. The coeffi cient of determination must satisfy the following:

This coeffi cient of determination represents the proportion of the sum of squares of y values’
devia-tions from their means that can be attributed to the linear relation between y and *x _{i}*.

**Analysis of the modulus of elasticity versus speci****fi**** c gravity**

Using the experiment’s data set and statistical regression analysis to establish a relation between
modulus of elasticity *E _{exp}* and specifi c gravity

*S*we obtained the following regression:

_{G} * E _{exp} = 160 + 11086 SG * (1)

The coeffi cient of determination *R-sq *is 28.1%. Table 2 shows the analysis of variance of the linear
regression.

From this analysis of the variance we can conclude that the regression is signifi cant. We can thus
reject the hypothesis *H _{0}* : β

*1 = 0*with a high level of confi dence. Figure 3 shows the regression plot.

Analyzing the prediction interval, we can, with 95% confi dence and prediction bands, observe that some results of the data did not adequately fi t in the model.

**Figure 3.** Regression Plot - Modulus of Elasticity and Specifi c Gravity Analysis of the modulus
of elasticity versus number of growth rings per inch.

Using the experimental data set, we analogously established a relation between modulus of elasti-city and the number of growth rings per inch per inch, and obtained the following regression:

*E _{exp} = 2947+ 88.6 RPI * (2)

where *E _{exp}* is the Young´s Modulus considering the three temperature conditions, and

*RPI*is the number of growth rings per inch per inch. The coeffi cient of determination is now

*R-sq*= 40.9%.

Table 4 shows the analysis of variance of the linear regression.

**Table 4.** Analysis of the Variance for Signifi cance of Regresion.

Analyzing the variance, we can conclude that the regression is signifi cant, and thus we can reject
the hypothesis *H _{0}* : β

*with a high level of confi dence.*

_{1}= 0Figure 4 illustrates the regression plot. Analyzing the prediction interval, we can, with 95% confi -dence and prediction bands, observe that some results of the data did not adequately fi t in the model. Similar to the earlier analysis, the linear regression cannot adequately model this relation, but we have a better adjustment to the adopted model.

**Figure 4.** Regression Plot - Modulus of Elasticity and the Number of growth rings per inch.

By adopting a quadratic polynomial model and cubic model, the coeffi cient of determination in the
results improved to *R-Sq* = 48.6% and *R-Sq* = 50.0%, respectively. On the other hand, the statistical test

*F _{0}* reached 24.91 for the quadratic model but only

*F*= 11.33 for the cubic model.

_{0}**Analysis of the Modulus of Elasticity versus Temperature Associated with Moisture Content**

The relationship between modulus of elasticity and temperature has been defi ned. In this study, we also associated the moisture contents of the specimens with three temperature conditions. From the statistical regression analysis we determined the following regression:

*E _{exp} = 5575 - 3.69 Temp - 124 MC * (3)

where *E _{exp}* is the Young´s Modulus Temp is the temperature and

*MC*the moisture contents. Table 5 shows the analysis of variance of the linear regression.

In this case, the coeffi cient of determination *R-sq* is 15.4%, a relatively low value. From this
analy-sis of the variance we can conclude that for *p* = 0%, the regression is signifi cant.

We can thus reject the hypothesis: with high level of confi dence.

*H _{0} : *β

*1 =*β

*2 = ... =*β

*k = 0 versus H1 :*β

*1*≠β

*2*≠

*... =*β

*k*≠

*0*with high level of confi dence

In Table 6, note that by using the Student’s t-distribution, we can estimate the infl uence that each parameter has on the Modulus of elasticity.

**Table 6. **Analysis of the Student´s *t* distribution

From this analysis of the variance we can conclude that, in terms of temperature, the regression is
not signifi cant (*p* is much greater than 15%) Thus, we cannot reject the hypothesis *H _{0} : *β

*1 = 0*with a

high level of confi dence.

Looking at the infl uence of moisture content, we can reject the null hypothesis at the 6.1% level of signifi cance, a satisfactory number for wood properties. These results are in accordance with the previous studies as before cited, such as Dinwoodie (2000).

**The Modulus of Elasticity versus Specifi c Gravity, the Number of growth rings per inch and **

**Temperature**

In this section, we perform a complete analysis of the infl uence on Young´s modulus of wood of the following parameters: moisture content, specifi c gravity, number of growth rings per inch and tem-perature associated with the moisture content.

We obtained the following regression:

*E _{exp} = 8455 - 11688 SG + 167 RPI - 7.16 Temp - 185 MC * (4)

Table 7 shows the analysis of variance of the linear regression.

The coeffi cient of determination is *R-sq* = 67.6%, a reasonable result for experimental data.

From this analysis of the variance we can conclude that for *p* = 0%, the regression is signifi cant.

This means that we can reject the hypothesis: with high level of confi dence.

*H _{0} : *β

*1 =*β

*2 = ... =*β

*k = 0 versus H1 :*β

*1*≠β

*2*≠

*... =*β

*k*≠

*0*with high level of confi dence

In Table 8, note that by using the Student’s t-distribution we can estimate the infl uence that each parameter has on the Modulus of elasticity.

**Table 8.** Analysis of the Student´s Distribution

From these results, we observe that the effect of the number of growth rings per inch is more sig-nifi cant than the effects of the other parameters. However, the moisture content effect is signifi cant, especially when interrelated with the temperature effects present in the analyzed model. The infl uences of temperature conditions and specifi c gravity on this model are negligible in the light of this wood sample and also of this current statistical procedure.

**Analysis of Speci****fi**** c Gravity versus Number of growth rings per inch**

Finally, we established a relation between specifi c gravity and the number of growth rings per inch, and adjusted the data through the following regression:

*SG = 0.278 + 0,00603 RPI * (5)

where *SG* is specifi c gravity and *RPI* is the number of rings per inch. Table 9 shows the analysis of
variance of the linear regression.

Figure 5 illustrates the regression plot. Analyzing the prediction interval, we can, with 95% confi -dence and prediction bands, observe that only a few results did not adequately adjust to the model.

**Figure 5.** Regression Plot - Specifi c Gravity and Number of growth rings per inch.

Examining the pertinent literature that contributes to a better understanding the current results,
we found, for instance, the study of Cramer *et al.* (2005). They demonstrated that the specifi c gravity
and the position of the ring on the cross section of earlywood and latewood of loblolly pine are strong
predictors of elastic modulus. In addition, they emphasized that biological and mechanical responses to
the environment are likely causes of variation in elastic modulus of earlywood and latewood.

Two other interesting articles and also consistent with these fi ndings were developed by Ballarin
and Palma (2003) and Rall *et al.*(2008), in which average results of elastic modulus of juvenile and
mature wood of *pinus taede* L. were evaluated. This piece of research revealed that the overall results
of the elastic modulus of juvenile wood were always smaller than that of mature wood, and that the
specifi c gravity and also the number of rings per inch were superior in the latter. A further established
issue was that the classifi cation of wood in density classes should be carried out using two different and
independent parameters: number of growth rings per inch and the latewood percentage.

These studies and our results evidenced the fact that specifi c gravity is a predictor of wood proper-ties, and provide arguments to indicate that the number of growth rings per inch may also be used as a predictor of wood properties.

**CONCLUSION**

In this study, we described the infl uence that several parameters have on changes in wood mechani-cal behavior by determining and analyzing the changes in the values of the modulus of elasticity. These parameters included specifi c gravity and number of growth rings per inch in three different temperature conditions.

Although many results presented in this research are well established, the literature does not pre-sent a complete study with a consistent statistical analyses focusing on the infl uence of the moisture content, the specifi c gravity, the number of annual growth ring and the temperature on the Young´s modulus of wood.

In this context, the most important conclusions that were drawn can be summarized as follows:

• The effect that the number of growth rings per inch has on the modulus of elasticity is relevant, especially when compared to the effects of specifi c gravity or temperature. Furthermore, this study proposes that the number of growth rings can serve as a good predictor of elastic modulus of wood.

• The specifi c gravity is less signifi cant, but we can affi rm that if the specifi c gravity increases, the modulus of elasticity also increases.

• The three different temperature conditions employed in this work changed the moisture content of the specimen, but did not signifi cantly affect the values of the modulus of elasticity.

We noted that the infl uence of the moisture content on the modulus of elasticity is signifi cant; if the moisture content increases, the modulus of elasticity decreases. However, we should also mention here that the moisture content effect is relative to the temperature effects present in the coupling.

It is important to emphasize that these conclusions are restricted to the current experimental data. To determine whether these results can be generalized, addition tests must be developed that take into account other species of wood, with different moisture content, specifi c gravity, number of growth rings per inch and temperature conditions.

**ACKNOWLEDGEMENTS**

The fi rst author would like to thank the Department of Civil and Environmental Engineering of the University of Wisconsin-Madison for assistance with material conditioning and offi ce space. Thanks also to FAPESP - Fundação de Amparo à Pesquisa do Estado de São Paulo/Brazil (#97/02710-0) and UNICAMP - State University of Campinas for fi nancial support during the sabbatical year in Madison, Wisconsin.

**REFERENCES**

**Ando, K.; Ohta, M. 1999.** Variability of fracture toughness by the crack tip position in an annual
ring of coniferous wood. *J Wood Sci* 45: 275–283.

**Ballarin, A . W.; Palma, H. A. L. 2003.** Rigidity and Strength Properties of pinus taeda L. Juvenile
And Mature timber. *Árvore* 27(3):371-380.

**Bodig, J.; Jayne, B.A. 1982. Mechanics of wood and wood composites.** Van Nostrand, New

York,

**Cramer, S.M.; Hermanson, J.C.; McMurtry, W.M. 1996.** Characterizing large strain crush

res-ponse of redwood. Sandia Report. SAND96 - 2966.UC-820, Sandia National Laboratories.

**Cramer, S.M.; Kretschmann, D.; Lakes, R.; Schmidt, T. 2005.** Earlywood and latewood elastic

properties in loblolly pine. *Holzforschung* 59:531-538.

**Dinwoodie, J.M. 2000. Timber - Its nature and behavior. **Van Nostrand Reinhold Company, New

York.

**Gerhards, C.C. 1982. **Effect of moisture content and temperature on mechanical properties of

wood: An analysis of immediate effects. *Wood and Fiber* 14(1): 443–449.

**Hermanson, J.C. 1996. **The triaxial behavior of redwood using a new confi ned compression
devi-ce. PhD thesis, Dept. of Civil Engr., Univ. of Wisconsin, Wisc.

**Hanhijiirvi, A. 2000. **Advances in the knowledge of the infl uence of moisture changes on the
long-term mechanical performance of timber structures. *Materials and Structures* 33: 43-49.

**Lenth, C.; Sargent, R. 2004. **Investigating the infl uence of moisture content and temperature on
the tensile stiffness of radiata pine. Proceedings of Third International Conference of the European
Society for wood Mechanics. UTAD, Vila Real, Portugal.

**Mascia, N. T. 2003.** Concerning the elastic orthotropic model applied to wood elastic properties.
Maderas. *Ciencia y tecnología* 5 (1):3-19.

**Montgomery, D.C.; Peck, E.A. 1992.***Introduction to linear regression analysis.* John Wiley &
Sons, Inc, New York.

**Rall, R.; Ballarin, A.W.; Palma, H.A.L. 2008.** Calssifi cation of the sawn wood of *pinus taeda *

L. in classes of density using digital processing of images. Proceedings of XI EBRAMEM. UEL, Lon-drina, Brazil.

**Ryan, B.F.; Joiner, B.L. 1994.***Minitab handbook.* Duxbury Press, Belmont, California.

**Wood Handbook 1987. Wood as an engineering material. **Agricultural Handbook 72. U.S. Dept.